#------------------------------------------------------------------------------
#$Date: 2016-03-25 14:32:06 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179900 $
#$URL: svn://www.crystallography.net/cod/cif/7/01/96/7019678.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7019678
loop_
_publ_author_name
'Zhang, Chun-Hua'
'Chen, Ya-Guang'
'Tang, Qun'
'Liu, Shu-Xia'
_publ_section_title
;
 Polynuclear complexes of main group and transition metals with
 polyaminopolycarboxylate and polyoxometalate.
;
_journal_issue                   33
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9971
_journal_page_last               9978
_journal_paper_doi               10.1039/c2dt12508k
_journal_volume                  41
_journal_year                    2012
_chemical_formula_sum            'C28 H68 N4 O82 Si W12 Zn5'
_chemical_formula_weight         4333.98
_chemical_name_systematic
;
?
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 122.324(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   36.118(4)
_cell_length_b                   11.4413(11)
_cell_length_c                   24.623(3)
_cell_measurement_reflns_used    500
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25
_cell_measurement_theta_min      3
_cell_volume                     8598.4(17)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       'w/ scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1025
_diffrn_reflns_av_sigmaI/netI    0.1181
_diffrn_reflns_limit_h_max       45
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       30
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            23688
_diffrn_reflns_theta_full        26.61
_diffrn_reflns_theta_max         26.61
_diffrn_reflns_theta_min         1.68
_diffrn_standards_interval_count 0
_exptl_absorpt_coefficient_mu    17.488
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.348
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             7888
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.09
_refine_diff_density_max         3.224
_refine_diff_density_min         -3.893
_refine_diff_density_rms         0.578
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.205
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     581
_refine_ls_number_reflns         8949
_refine_ls_number_restraints     125
_refine_ls_restrained_S_all      1.198
_refine_ls_R_factor_all          0.1484
_refine_ls_R_factor_gt           0.1164
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+3792.8342P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2439
_refine_ls_wR_factor_ref         0.2558
_reflns_number_gt                6654
_reflns_number_total             8949
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt12508k.txt
_cod_data_source_block           Zn
_cod_original_cell_volume        8598.4(16)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7019678
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 0.14111(4) 0.34171(12) 0.39819(7) 0.0216(3) Uani 1 1 d .
W2 W 0.31225(4) 0.16835(13) 0.43458(7) 0.0215(3) Uani 1 1 d .
W3 W 0.16910(4) 0.04519(15) 0.39984(7) 0.0302(4) Uani 1 1 d .
W4 W 0.21598(4) 0.03474(15) 0.56798(7) 0.0285(4) Uani 1 1 d .
W5 W 0.20294(5) 0.25817(13) 0.33189(6) 0.0249(3) Uani 1 1 d .
W6 W 0.27812(5) -0.04741(14) 0.50208(7) 0.0275(4) Uani 1 1 d .
O1W O 0.3674(8) -0.306(2) 0.3794(12) 0.035(6) Uani 1 1 d .
H21A H 0.3570 -0.2893 0.3352 0.053 Uiso 1 1 d R
H21B H 0.3796 -0.3833 0.3898 0.053 Uiso 1 1 d R
O1 O 0.1369(14) 0.182(4) 0.395(2) 0.084(13) Uani 1 1 d U
OW1 O 0.381(3) 0.299(9) 0.055(4) 0.11(3) Uiso 0.50 1 d PD
OW1A O 0.373(6) 0.261(17) -0.004(8) 0.21(7) Uiso 0.50 1 d P
O2W O 0.4432(11) -0.301(4) 0.5170(16) 0.078(14) Uani 1 1 d .
H22B H 0.4206 -0.3200 0.5248 0.117 Uiso 1 1 d R
H22C H 0.4515 -0.3702 0.5040 0.117 Uiso 1 1 d R
OW2 O 0.4459(19) 0.795(6) 0.297(3) 0.037(13) Uiso 0.50 1 d P
OW2A O 0.427(2) 0.758(6) 0.285(3) 0.041(14) Uiso 0.50 1 d P
O3W O 0.4602(10) -0.247(4) 0.4180(12) 0.057(10) Uani 1 1 d .
H23A H 0.4873 -0.2044 0.4403 0.086 Uiso 1 1 d R
H23B H 0.4655 -0.3275 0.4305 0.086 Uiso 1 1 d R
O3 O 0.1688(16) 0.334(5) 0.355(2) 0.026(11) Uiso 0.50 1 d P
O3A O 0.1481(16) 0.329(5) 0.320(3) 0.028(11) Uiso 0.50 1 d P
OW3 O 0.4498(11) 0.124(3) 0.5587(19) 0.070(11) Uani 1 1 d .
O4W O 0.475(2) -0.078(7) 0.522(3) 0.053(18) Uiso 0.50 1 d P
H24B H 0.4588 -0.0282 0.5399 0.079 Uiso 1 1 d R
O4WA O 0.462(2) -0.042(7) 0.494(4) 0.07(2) Uiso 0.50 1 d P
H24A H 0.4745 -0.0131 0.4920 0.098 Uiso 1 1 d R
OW4 O 0.5033(8) -0.046(3) 0.3010(13) 0.036(6) Uani 1 1 d U
O5W O 0.4610(11) 0.401(4) 0.1811(16) 0.069(12) Uani 1 1 d .
H25A H 0.4754 0.3782 0.1594 0.104 Uiso 1 1 d R
H25B H 0.4593 0.3350 0.2038 0.104 Uiso 1 1 d R
OW5 O 0.4221(11) 0.479(4) 0.5541(19) 0.088(15) Uani 1 1 d .
O6W O 0.4657(11) 0.661(3) 0.1833(17) 0.064(10) Uani 1 1 d .
H26A H 0.4771 0.7355 0.2033 0.095 Uiso 1 1 d R
H26B H 0.4696 0.6521 0.1479 0.095 Uiso 1 1 d R
O7 O 0.1824(9) 0.160(4) 0.565(2) 0.090(15) Uani 1 1 d .
O7W O 0.3816(12) -0.119(4) 0.4771(18) 0.072(10) Uani 1 1 d U
H27A H 0.3964 -0.0579 0.5083 0.108 Uiso 1 1 d R
H27B H 0.3541 -0.0901 0.4423 0.108 Uiso 1 1 d R
O9 O 0.1301(8) -0.050(3) 0.3538(13) 0.036(6) Uani 1 1 d U
O9W O 0.506(2) 0.174(6) 0.360(3) 0.16(2) Uiso 1 1 d .
H29A H 0.5071 0.2317 0.3325 0.188 Uiso 1 1 d R
H29B H 0.5223 0.2106 0.4018 0.188 Uiso 1 1 d R
O10 O 0.4561(7) 0.544(2) 0.2806(13) 0.030(6) Uani 1 1 d .
O11 O 0.4690(7) 0.301(3) 0.4260(12) 0.038(7) Uani 1 1 d .
O12 O 0.3865(11) -0.081(3) 0.3622(16) 0.063(10) Uani 1 1 d .
O14 O 0.2907(11) -0.187(3) 0.5027(13) 0.048(8) Uani 1 1 d .
O16 O 0.1819(10) 0.259(3) 0.2513(14) 0.055(9) Uani 1 1 d .
O17 O 0.1743(9) 0.017(5) 0.4808(14) 0.11(2) Uani 1 1 d .
O18 O 0.2560(11) 0.180(3) 0.3588(17) 0.063(9) Uani 1 1 d U
O19 O 0.2556(11) -0.050(5) 0.5576(13) 0.097(18) Uani 1 1 d .
O20 O 0.2148(11) 0.324(3) 0.4959(18) 0.009(8) Uani 0.50 1 d PU
O21 O 0.1772(13) 0.115(4) 0.3347(19) 0.074(11) Uani 1 1 d U
O22 O 0.3422(9) 0.133(3) 0.4028(14) 0.047(9) Uani 1 1 d .
O23 O 0.1439(10) 0.327(3) 0.4776(11) 0.047(8) Uani 1 1 d .
O24 O 0.2644(9) 0.096(3) 0.6434(17) 0.055(9) Uani 1 1 d .
O25 O 0.0883(9) 0.378(3) 0.3491(15) 0.054(9) Uani 1 1 d .
O26 O 0.4255(10) 0.087(3) 0.3804(16) 0.053(8) Uani 1 1 d .
O27 O 0.2339(14) 0.108(4) 0.497(2) 0.021(10) Uiso 0.50 1 d P
O28 O 0.1696(9) 0.479(3) 0.4268(14) 0.042(7) Uiso 1 1 d .
O29 O 0.2982(10) 0.017(3) 0.4489(11) 0.053(10) Uani 1 1 d .
O30 O 0.4485(8) 0.357(3) 0.2865(14) 0.045(8) Uani 1 1 d .
O31 O 0.1982(8) -0.069(2) 0.5985(12) 0.030(6) Uiso 1 1 d .
O32 O 0.4577(9) 0.355(3) 0.5026(12) 0.039(7) Uani 1 1 d .
O36 O 0.2579(11) 0.273(3) 0.4414(17) 0.007(7) Uiso 0.50 1 d P
O38 O 0.416(2) 0.145(7) 0.171(3) 0.19(3) Uani 1 1 d DU
O39 O 0.4410(19) 0.111(6) 0.262(3) 0.13(2) Uani 1 1 d U
O40 O 0.2045(12) 0.237(4) 0.4291(18) 0.010(8) Uani 0.50 1 d PU
O41 O 0.2195(12) -0.036(4) 0.4283(17) 0.069(10) Uani 1 1 d U
C1 C 0.4404(10) 0.455(3) 0.2928(18) 0.025(8) Uani 1 1 d .
C2 C 0.4132(10) 0.485(3) 0.3213(18) 0.024(8) Uani 1 1 d .
H2A H 0.4319 0.5231 0.3624 0.028 Uiso 1 1 calc R
H2B H 0.3905 0.5396 0.2931 0.028 Uiso 1 1 calc R
C3 C 0.3140(9) 0.437(4) 0.2788(15) 0.037(11) Uani 1 1 d D
H3A H 0.3138 0.4144 0.3165 0.044 Uiso 1 1 calc R
H3B H 0.3232 0.5180 0.2840 0.044 Uiso 1 1 calc R
C4 C 0.3987(10) 0.380(3) 0.3922(15) 0.022(7) Uani 1 1 d U
H4A H 0.3776 0.3261 0.3913 0.027 Uiso 1 1 calc R
H4B H 0.3931 0.4568 0.4027 0.027 Uiso 1 1 calc R
C5 C 0.2533(14) 0.304(5) 0.205(2) 0.055(14) Uani 1 1 d .
H5A H 0.2251 0.3018 0.1648 0.066 Uiso 1 1 calc R
H5B H 0.2496 0.2727 0.2384 0.066 Uiso 1 1 calc R
C6 C 0.3468(12) 0.363(4) 0.275(2) 0.042(10) Uani 1 1 d DU
H6A H 0.3465 0.3902 0.2369 0.051 Uiso 1 1 calc R
C7 C 0.3317(9) 0.240(3) 0.2608(14) 0.025(7) Uiso 1 1 d D
H7A H 0.3297 0.2093 0.2964 0.030 Uiso 1 1 calc R
C8 C 0.2684(10) 0.426(5) 0.221(2) 0.075(19) Uani 1 1 d D
H8A H 0.2485 0.4699 0.2281 0.091 Uiso 1 1 calc R
H8B H 0.2676 0.4614 0.1841 0.091 Uiso 1 1 calc R
C9 C 0.2881(9) 0.224(3) 0.1991(14) 0.031(9) Uani 1 1 d D
H9A H 0.2793 0.1425 0.1931 0.037 Uiso 1 1 calc R
H9B H 0.2898 0.2488 0.1628 0.037 Uiso 1 1 calc R
C10 C 0.4461(11) 0.340(3) 0.4459(16) 0.024(7) Uani 1 1 d U
C11 C 0.3935(12) 0.014(4) 0.3432(19) 0.033(9) Uani 1 1 d U
C12 C 0.3617(14) 0.048(4) 0.273(2) 0.043(10) Uani 1 1 d U
H12A H 0.3659 -0.0044 0.2456 0.051 Uiso 1 1 calc R
H12B H 0.3319 0.0384 0.2623 0.051 Uiso 1 1 calc R
C14 C 0.4102(13) 0.139(5) 0.213(3) 0.061(14) Uani 1 1 d DU
C15 C 0.3656(11) 0.175(4) 0.1975(17) 0.033(8) Uani 1 1 d DU
H15A H 0.3586 0.2532 0.1796 0.039 Uiso 1 1 calc R
H15B H 0.3434 0.1215 0.1666 0.039 Uiso 1 1 calc R
N1 N 0.3927(8) 0.383(3) 0.3308(12) 0.018(6) Uani 1 1 d U
N2 N 0.3673(9) 0.171(3) 0.2578(15) 0.035(8) Uani 1 1 d .
Zn1 Zn 0.43115(13) 0.2285(4) 0.3333(2) 0.0287(9) Uani 1 1 d .
Zn2 Zn 0.41815(17) -0.1795(5) 0.4417(2) 0.0409(12) Uani 1 1 d .
Zn3 Zn 0.5000 0.5301(5) 0.2500 0.0279(13) Uani 1 2 d S
Si1 Si 0.2500 0.2500 0.5000 0.023(3) Uani 1 2 d SU
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O25 W1 O28 105.0(15) . .
O25 W1 O3 111(2) . .
O28 W1 O3 84.0(19) . .
O25 W1 O1 100.3(17) . .
O28 W1 O1 154.6(16) . .
O3 W1 O1 89(2) . .
O25 W1 O23 100.2(16) . .
O28 W1 O23 88.3(12) . .
O3 W1 O23 148.7(19) . .
O1 W1 O23 85.1(16) . .
O25 W1 O3A 90.3(19) . .
O28 W1 O3A 95.4(17) . .
O3 W1 O3A 21.7(17) . .
O1 W1 O3A 87(2) . .
O23 W1 O3A 167.7(18) . .
O25 W1 O40 155.1(16) . .
O28 W1 O40 93.7(13) . .
O3 W1 O40 53.9(19) . .
O1 W1 O40 62.9(16) . .
O23 W1 O40 96.7(14) . .
O3A W1 O40 71.4(17) . .
O25 W1 O20 160.8(16) . .
O28 W1 O20 66.1(13) . .
O3 W1 O20 85.6(18) . .
O1 W1 O20 89.0(16) . .
O23 W1 O20 63.6(13) . .
O3A W1 O20 107.2(16) . .
O40 W1 O20 43.7(13) . .
O22 W2 O23 100.7(15) . 7_556
O22 W2 O18 100.1(15) . .
O23 W2 O18 159.2(15) 7_556 .
O22 W2 O29 99.6(16) . .
O23 W2 O29 87.4(11) 7_556 .
O18 W2 O29 89.6(14) . .
O22 W2 O7 98.9(17) . 7_556
O23 W2 O7 87.1(15) 7_556 7_556
O18 W2 O7 89.2(15) . 7_556
O29 W2 O7 161.4(17) . 7_556
O22 W2 O36 155.5(15) . .
O23 W2 O36 97.2(14) 7_556 .
O18 W2 O36 62.8(14) . .
O29 W2 O36 97.7(15) . .
O7 W2 O36 65.3(14) 7_556 .
O22 W2 O20 162.0(16) . 7_556
O23 W2 O20 65.8(13) 7_556 7_556
O18 W2 O20 93.9(14) . 7_556
O29 W2 O20 69.1(14) . 7_556
O7 W2 O20 92.4(16) 7_556 7_556
O36 W2 O20 42.4(13) . 7_556
O9 W3 O41 103.5(16) . .
O9 W3 O1 103.3(16) . .
O41 W3 O1 153.2(19) . .
O9 W3 O17 100.1(18) . .
O41 W3 O17 89.6(15) . .
O1 W3 O17 85.3(19) . .
O9 W3 O21 98.8(15) . .
O41 W3 O21 88.1(17) . .
O1 W3 O21 88.2(18) . .
O17 W3 O21 161(2) . .
O9 W3 O27 154.1(15) . .
O41 W3 O27 61.6(16) . .
O1 W3 O27 93.2(17) . .
O17 W3 O27 61.0(16) . .
O21 W3 O27 101.6(16) . .
O9 W3 O40 155.6(13) . .
O41 W3 O40 95.1(16) . .
O1 W3 O40 59.4(16) . .
O17 W3 O40 95.5(19) . .
O21 W3 O40 65.8(15) . .
O27 W3 O40 50.1(14) . .
O31 W4 O17 99.9(19) . .
O31 W4 O7 99.2(17) . .
O17 W4 O7 86.1(19) . .
O31 W4 O19 101.4(19) . .
O17 W4 O19 89.6(14) . .
O7 W4 O19 159(2) . .
O31 W4 O24 101.3(14) . .
O17 W4 O24 159(2) . .
O7 W4 O24 89.4(13) . .
O19 W4 O24 87.3(14) . .
O31 W4 O27 155.0(15) . .
O17 W4 O27 63.1(17) . .
O7 W4 O27 98(2) . .
O19 W4 O27 62.5(19) . .
O24 W4 O27 97.1(16) . .
O31 W4 O36 157.0(12) . 7_556
O17 W4 O36 96(2) . 7_556
O7 W4 O36 65.1(15) . 7_556
O19 W4 O36 95.4(19) . 7_556
O24 W4 O36 63.6(13) . 7_556
O27 W4 O36 48.0(14) . 7_556
O16 W5 O3 113.7(19) . .
O16 W5 O18 98.5(15) . .
O3 W5 O18 147.7(19) . .
O16 W5 O21 97.0(17) . .
O3 W5 O21 88(2) . .
O18 W5 O21 90.0(17) . .
O16 W5 O24 100.4(17) . 7_556
O3 W5 O24 83.9(18) . 7_556
O18 W5 O24 88.1(14) . 7_556
O21 W5 O24 162.5(16) . 7_556
O16 W5 O3A 92.4(18) . .
O3 W5 O3A 22.5(17) . .
O18 W5 O3A 168.1(18) . .
O21 W5 O3A 83.7(19) . .
O24 W5 O3A 94.8(17) 7_556 .
O16 W5 O36 156.0(14) . .
O3 W5 O36 84.8(18) . .
O18 W5 O36 63.6(14) . .
O21 W5 O36 98.7(15) . .
O24 W5 O36 65.0(14) 7_556 .
O3A W5 O36 107.2(17) . .
O16 W5 O40 158.3(15) . .
O3 W5 O40 52.7(18) . .
O18 W5 O40 97.2(14) . .
O21 W5 O40 67.9(15) . .
O24 W5 O40 95.1(15) 7_556 .
O3A W5 O40 71.0(17) . .
O36 W5 O40 45.7(12) . .
O14 W6 O41 103.4(17) . .
O14 W6 O28 104.6(15) . 7_556
O41 W6 O28 152.0(16) . 7_556
O14 W6 O19 101(2) . .
O41 W6 O19 90.2(14) . .
O28 W6 O19 86.7(14) 7_556 .
O14 W6 O29 99.8(15) . .
O41 W6 O29 87.6(14) . .
O28 W6 O29 85.5(11) 7_556 .
O19 W6 O29 159(2) . .
O14 W6 O27 154.9(16) . .
O41 W6 O27 61.5(16) . .
O28 W6 O27 92.9(14) 7_556 .
O19 W6 O27 61.4(19) . .
O29 W6 O27 99.4(16) . .
Zn2 O1W H21A 109.6 . .
Zn2 O1W H21B 109.2 . .
H21A O1W H21B 109.5 . .
W1 O1 W3 141(2) . .
OW1 OW1A O7W 126(10) . 6
Zn2 O2W H22B 108.5 . .
Zn2 O2W H22C 108.4 . .
H22B O2W H22C 109.5 . .
Zn2 O3W H23A 109.4 . .
Zn2 O3W H23B 108.8 . .
H23A O3W H23B 109.5 . .
O3A O3 W1 98(6) . .
O3A O3 W5 93(6) . .
W1 O3 W5 152(3) . .
O3 O3A W5 65(5) . .
O3 O3A W1 61(5) . .
W5 O3A W1 120(3) . .
O4WA O4W Zn2 68(9) . .
O4WA O4W H24B 81.3 . .
Zn2 O4W H24B 100.2 . .
O4WA O4W H24A 32.4 . .
Zn2 O4W H24A 94.0 . .
H24B O4W H24A 95.6 . .
O4W O4WA Zn2 93(10) . .
O4W O4WA H24B 62.1 . .
Zn2 O4WA H24B 104.5 . .
O4W O4WA H24A 105.7 . .
Zn2 O4WA H24A 136.3 . .
H24B O4WA H24A 119.1 . .
Zn3 O5W H25A 108.1 . .
Zn3 O5W H25B 107.7 . .
H25A O5W H25B 109.5 . .
Zn3 O6W H26A 108.9 . .
Zn3 O6W H26B 109.1 . .
H26A O6W H26B 109.5 . .
W4 O7 W2 135(2) . 7_556
OW1A O7W Zn2 92(6) 6_556 .
OW1A O7W H27A 124.1 6_556 .
Zn2 O7W H27A 112.2 . .
OW1A O7W H27B 107.8 6_556 .
Zn2 O7W H27B 109.3 . .
H27A O7W H27B 109.5 . .
H29A O9W H29B 103.3 . .
C1 O10 Zn3 123(2) . .
C10 O11 Zn1 113(2) . .
C11 O12 Zn2 136(3) . .
W4 O17 W3 138(2) . .
W5 O18 W2 137(2) . .
W4 O19 W6 137(3) . .
Si1 O20 O36 60.8(19) . 7_556
Si1 O20 O40 59.5(17) . .
O36 O20 O40 102(3) 7_556 .
Si1 O20 W2 129(2) . 7_556
O36 O20 W2 68.6(17) 7_556 7_556
O40 O20 W2 136(2) . 7_556
Si1 O20 W1 123(2) . .
O36 O20 W1 137(2) 7_556 .
O40 O20 W1 63.9(16) . .
W2 O20 W1 93.1(12) 7_556 .
W5 O21 W3 132(2) . .
W2 O23 W1 136.6(18) 7_556 .
W4 O24 W5 136.1(19) . 7_556
C11 O26 Zn1 115(3) . .
Si1 O27 W4 122(2) . .
Si1 O27 W6 121(2) . .
W4 O27 W6 98.1(17) . .
Si1 O27 W3 117(2) . .
W4 O27 W3 97.3(16) . .
W6 O27 W3 96.0(17) . .
W1 O28 W6 141.9(17) . 7_556
W2 O29 W6 135(2) . .
C1 O30 Zn1 114(3) . .
Si1 O36 O20 52.4(16) . 7_556
Si1 O36 W5 124.1(18) . .
O20 O36 W5 135(2) 7_556 .
Si1 O36 W2 121.3(19) . .
O20 O36 W2 68.9(17) 7_556 .
W5 O36 W2 96.0(13) . .
Si1 O36 W4 119.1(19) . 7_556
O20 O36 W4 127(2) 7_556 7_556
W5 O36 W4 95.1(13) . 7_556
W2 O36 W4 94.1(12) . 7_556
C14 O39 Zn1 99(4) . .
Si1 O40 O20 51.2(16) . .
Si1 O40 W1 124(2) . .
O20 O40 W1 72.4(17) . .
Si1 O40 W5 122.1(19) . .
O20 O40 W5 139(3) . .
W1 O40 W5 97.4(14) . .
Si1 O40 W3 118(2) . .
O20 O40 W3 126(2) . .
W1 O40 W3 95.6(13) . .
W5 O40 W3 93.9(13) . .
W3 O41 W6 140(2) . .
O30 C1 O10 123(3) . .
O30 C1 C2 123(3) . .
O10 C1 C2 114(3) . .
N1 C2 C1 114(3) . .
N1 C2 H2A 108.8 . .
C1 C2 H2A 108.8 . .
N1 C2 H2B 108.8 . .
C1 C2 H2B 108.8 . .
H2A C2 H2B 107.7 . .
C8 C3 C6 113(3) . .
C8 C3 H3A 108.9 . .
C6 C3 H3A 108.9 . .
C8 C3 H3B 108.9 . .
C6 C3 H3B 108.9 . .
H3A C3 H3B 107.7 . .
N1 C4 C10 113(3) . .
N1 C4 H4A 109.1 . .
C10 C4 H4A 109.1 . .
N1 C4 H4B 109.1 . .
C10 C4 H4B 109.1 . .
H4A C4 H4B 107.8 . .
C8 C5 C9 111(4) . .
C8 C5 H5A 109.4 . .
C9 C5 H5A 109.4 . .
C8 C5 H5B 109.4 . .
C9 C5 H5B 109.4 . .
H5A C5 H5B 108.0 . .
C7 C6 N1 117(3) . .
C7 C6 C3 110(4) . .
N1 C6 C3 112(3) . .
C7 C6 H6A 105.6 . .
N1 C6 H6A 105.6 . .
C3 C6 H6A 105.6 . .
C6 C7 C9 114(3) . .
C6 C7 N2 106(3) . .
C9 C7 N2 110(3) . .
C6 C7 H7A 108.8 . .
C9 C7 H7A 108.8 . .
N2 C7 H7A 108.8 . .
C5 C8 C3 113(4) . .
C5 C8 H8A 109.0 . .
C3 C8 H8A 109.0 . .
C5 C8 H8B 109.0 . .
C3 C8 H8B 109.0 . .
H8A C8 H8B 107.8 . .
C7 C9 C5 106(3) . .
C7 C9 H9A 110.5 . .
C5 C9 H9A 110.5 . .
C7 C9 H9B 110.5 . .
C5 C9 H9B 110.5 . .
H9A C9 H9B 108.6 . .
O32 C10 O11 126(3) . .
O32 C10 C4 118(3) . .
O11 C10 C4 115(3) . .
O12 C11 O26 124(4) . .
O12 C11 C12 117(4) . .
O26 C11 C12 118(4) . .
N2 C12 C11 113(3) . .
N2 C12 H12A 108.9 . .
C11 C12 H12A 108.9 . .
N2 C12 H12B 108.9 . .
C11 C12 H12B 108.9 . .
H12A C12 H12B 107.7 . .
O38 C14 O39 114(5) . .
O38 C14 C15 116(6) . .
O39 C14 C15 130(5) . .
N2 C15 C14 106(3) . .
N2 C15 H15A 110.5 . .
C14 C15 H15A 110.5 . .
N2 C15 H15B 110.5 . .
C14 C15 H15B 110.5 . .
H15A C15 H15B 108.7 . .
C4 N1 C2 113(3) . .
C4 N1 C6 116(3) . .
C2 N1 C6 113(3) . .
C4 N1 Zn1 102(2) . .
C2 N1 Zn1 105.8(18) . .
C6 N1 Zn1 105.3(19) . .
C15 N2 C12 110(3) . .
C15 N2 C7 117(3) . .
C12 N2 C7 104(3) . .
C15 N2 Zn1 108(2) . .
C12 N2 Zn1 107(2) . .
C7 N2 Zn1 110(2) . .
O26 Zn1 O11 84.4(13) . .
O26 Zn1 N2 82.1(13) . .
O11 Zn1 N2 146.3(10) . .
O26 Zn1 O30 168.2(12) . .
O11 Zn1 O30 96.0(12) . .
N2 Zn1 O30 103.3(11) . .
O26 Zn1 N1 113.1(11) . .
O11 Zn1 N1 75.5(9) . .
N2 Zn1 N1 81.7(11) . .
O30 Zn1 N1 78.4(11) . .
O26 Zn1 O39 94.0(18) . .
O11 Zn1 O39 139.1(15) . .
N2 Zn1 O39 72.8(16) . .
O30 Zn1 O39 77.9(18) . .
N1 Zn1 O39 139.7(17) . .
O12 Zn2 O3W 93.2(14) . .
O12 Zn2 O7W 93.6(16) . .
O3W Zn2 O7W 172.8(13) . .
O12 Zn2 O2W 171.1(16) . .
O3W Zn2 O2W 88.1(13) . .
O7W Zn2 O2W 85.4(15) . .
O12 Zn2 O4WA 92(2) . .
O3W Zn2 O4WA 91(2) . .
O7W Zn2 O4WA 86(2) . .
O2W Zn2 O4WA 97(3) . .
O12 Zn2 O1W 82.1(12) . .
O3W Zn2 O1W 91.3(13) . .
O7W Zn2 O1W 92.0(14) . .
O2W Zn2 O1W 89.1(15) . .
O4WA Zn2 O1W 173(2) . .
O12 Zn2 O4W 110(2) . .
O3W Zn2 O4W 88(2) . .
O7W Zn2 O4W 87(2) . .
O2W Zn2 O4W 79(2) . .
O4WA Zn2 O4W 19(2) . .
O1W Zn2 O4W 168(2) . .
O6W Zn3 O6W 88(2) 2_655 .
O6W Zn3 O10 84.6(12) 2_655 .
O6W Zn3 O10 89.1(11) . .
O6W Zn3 O10 89.1(11) 2_655 2_655
O6W Zn3 O10 84.6(12) . 2_655
O10 Zn3 O10 171.3(14) . 2_655
O6W Zn3 O5W 176.1(14) 2_655 .
O6W Zn3 O5W 90.6(16) . .
O10 Zn3 O5W 92.0(11) . .
O10 Zn3 O5W 94.1(10) 2_655 .
O6W Zn3 O5W 90.6(16) 2_655 2_655
O6W Zn3 O5W 176.1(15) . 2_655
O10 Zn3 O5W 94.1(10) . 2_655
O10 Zn3 O5W 92.0(11) 2_655 2_655
O5W Zn3 O5W 92(2) . 2_655
O20 Si1 O20 180(3) . 7_556
O20 Si1 O36 113(2) . .
O20 Si1 O36 67(2) 7_556 .
O20 Si1 O36 67(2) . 7_556
O20 Si1 O36 113(2) 7_556 7_556
O36 Si1 O36 180(2) . 7_556
O20 Si1 O40 110.7(19) . 7_556
O20 Si1 O40 69.3(19) 7_556 7_556
O36 Si1 O40 112.0(18) . 7_556
O36 Si1 O40 68.0(18) 7_556 7_556
O20 Si1 O40 69.3(19) . .
O20 Si1 O40 110.7(19) 7_556 .
O36 Si1 O40 68.0(18) . .
O36 Si1 O40 112.0(18) 7_556 .
O40 Si1 O40 180(3) 7_556 .
O20 Si1 O27 74(2) . 7_556
O20 Si1 O27 106(2) 7_556 7_556
O36 Si1 O27 71(2) . 7_556
O36 Si1 O27 109(2) 7_556 7_556
O40 Si1 O27 75(2) 7_556 7_556
O40 Si1 O27 105(2) . 7_556
O20 Si1 O27 106(2) . .
O20 Si1 O27 74(2) 7_556 .
O36 Si1 O27 109(2) . .
O36 Si1 O27 71(2) 7_556 .
O40 Si1 O27 105(2) 7_556 .
O40 Si1 O27 75(2) . .
O27 Si1 O27 180(3) 7_556 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O25 1.67(3) .
W1 O28 1.80(3) .
W1 O3 1.82(5) .
W1 O1 1.84(5) .
W1 O23 1.91(3) .
W1 O3A 2.07(5) .
W1 O40 2.32(4) .
W1 O20 2.46(4) .
W2 O22 1.69(2) .
W2 O23 1.88(2) 7_556
W2 O18 1.89(3) .
W2 O29 1.89(3) .
W2 O7 1.97(4) 7_556
W2 O36 2.38(4) .
W2 O20 2.39(4) 7_556
W3 O9 1.66(3) .
W3 O41 1.82(4) .
W3 O1 1.91(5) .
W3 O17 1.93(3) .
W3 O21 1.95(4) .
W3 O27 2.39(4) .
W3 O40 2.45(4) .
W4 O31 1.70(3) .
W4 O17 1.86(3) .
W4 O7 1.86(4) .
W4 O19 1.86(4) .
W4 O24 1.88(3) .
W4 O27 2.33(4) .
W4 O36 2.45(4) 7_556
W5 O16 1.70(3) .
W5 O3 1.82(5) .
W5 O18 1.89(3) .
W5 O21 1.90(4) .
W5 O24 1.94(3) 7_556
W5 O3A 2.02(5) .
W5 O36 2.35(3) .
W5 O40 2.38(4) .
W6 O14 1.65(3) .
W6 O41 1.92(4) .
W6 O28 1.92(3) 7_556
W6 O19 1.93(4) .
W6 O29 1.95(3) .
W6 O27 2.34(5) .
O1W Zn2 2.19(3) .
O1W H21A 0.9605 .
O1W H21B 0.9599 .
OW1 OW1A 1.40(18) .
OW1A O7W 1.77(19) 6
O2W Zn2 2.10(3) .
O2W H22B 0.9595 .
O2W H22C 0.9603 .
OW2 OW2A 0.71(7) .
O3W Zn2 2.05(3) .
O3W H23A 0.9600 .
O3W H23B 0.9598 .
O3 O3A 0.77(5) .
O4W O4WA 0.72(9) .
O4W Zn2 2.28(7) .
O4W H24B 1.0744 .
O4W H24A 1.0443 .
O4WA Zn2 2.12(8) .
O4WA H24B 1.2015 .
O4WA H24A 0.5815 .
O5W Zn3 2.12(3) .
O5W H25A 0.9598 .
O5W H25B 0.9605 .
O6W Zn3 2.07(3) .
O6W H26A 0.9600 .
O6W H26B 0.9599 .
O7 W2 1.97(4) 7_556
O7W OW1A 1.77(19) 6_556
O7W Zn2 2.05(3) .
O7W H27A 0.9597 .
O7W H27B 0.9596 .
O9W H29A 0.9598 .
O9W H29B 0.9602 .
O10 C1 1.28(4) .
O10 Zn3 2.09(2) .
O11 C10 1.25(4) .
O11 Zn1 2.11(3) .
O12 C11 1.26(5) .
O12 Zn2 2.01(3) .
O20 Si1 1.49(4) .
O20 O36 1.72(5) 7_556
O20 O40 1.78(5) .
O20 W2 2.39(4) 7_556
O23 W2 1.88(2) 7_556
O24 W5 1.94(3) 7_556
O26 C11 1.31(5) .
O26 Zn1 2.07(3) .
O27 Si1 1.72(5) .
O28 W6 1.92(3) 7_556
O30 C1 1.19(5) .
O30 Zn1 2.16(3) .
O32 C10 1.24(4) .
O36 Si1 1.64(4) .
O36 O20 1.72(5) 7_556
O36 W4 2.45(4) 7_556
O38 C14 1.16(8) .
O39 C14 1.16(7) .
O39 Zn1 2.39(6) .
O40 Si1 1.64(4) .
C1 C2 1.52(5) .
C2 N1 1.46(4) .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
C3 C8 1.502(10) .
C3 C6 1.503(10) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 N1 1.41(4) .
C4 C10 1.57(4) .
C4 H4A 0.9700 .
C4 H4B 0.9700 .
C5 C8 1.48(7) .
C5 C9 1.63(6) .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 C7 1.48(5) .
C6 N1 1.50(5) .
C6 H6A 0.9800 .
C7 C9 1.504(10) .
C7 N2 1.54(4) .
C7 H7A 0.9800 .
C8 H8A 0.9700 .
C8 H8B 0.9700 .
C9 H9A 0.9700 .
C9 H9B 0.9700 .
C11 C12 1.53(5) .
C12 N2 1.49(6) .
C12 H12A 0.9700 .
C12 H12B 0.9700 .
C14 C15 1.501(10) .
C15 N2 1.45(5) .
C15 H15A 0.9700 .
C15 H15B 0.9700 .
N1 Zn1 2.23(3) .
N2 Zn1 2.15(3) .
Zn3 O6W 2.07(3) 2_655
Zn3 O10 2.09(2) 2_655
Zn3 O5W 2.12(3) 2_655
Si1 O20 1.49(4) 7_556
Si1 O36 1.64(4) 7_556
Si1 O40 1.64(4) 7_556
Si1 O27 1.72(5) 7_556
